A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE


 Erin Todd
 11 months ago
 Views:
Transcription
1 A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering, The University of Manchester, Manchester M6 QD, U.K. SUMMARY Strain induced damage modes and their interactions are modelled using the finite element method for CMC tows and º/9º laminates. For both situations, biaxial straining is addressed, together with the degradation of Young s moduli and Poisson s ratios. In all cases, the expected stressstrain behaviour is predicted. Keywords: CMCs; Tows; Finite Element Method; Damage Mechanisms; Orthotropic Material; Constitutive Equations INTRODUCTION The superior material properties of Ceramic Matrix Composites (CMCs), e.g. low density and good mechanical and thermal properties at high temperatures make them favourable materials for use in: rocket nozzles; thermal protection systems; and gas turbine engines []. To perform optimal design of these engineering components, a highly efficient yet computational accurate model is a necessary requirement, due to the complex spatial topology and interactive damage mechanisms of woven CMCs. A finite element (FE) model of a unit cell geometry is a commonly used approach to study the behaviour of CMCs. Sheikh et al. [] employed a microstructural FE model to predict steadystate and transient heat conduction for the plain weave DLRXT composite. Deepak and Whitcomb [] evaluated load flow in plain weave composites by using a detailed D FE model and a nonstandard postprocessing technique. Although the full FE analysis is capable of predicting accurate micromechanical responses, it is computationally expensive because a precise description of the geometry is required. In order to tackle practical problems in the design and analysis of composites, some computationally efficient FE models have been developed. Tanov and Tabiei [4] predicted the equivalent material properties of plain weave fabric composites by homogenising an entire unit cell model. Cox et al. [5] introduced a Binary Model, which is composed of two virtual components: a D truss element and a D solid element. Whilst the Binary Model has great simplicity, it does require accurate determination of the mechanical and thermal properties of the two virtual components.
2 However, an alternative simpler and more accurate approach has been adopted here. For all of these approaches, the material properties are assumed to be linear elastic. The present paper addresses the development of a conceptually simple and computationally economic FE model, which emphasises the effects of straininduced damage modes and their interactions on the mechanical behaviour. Nonlinear material properties are modelled by multilinear elastic discretisation. A unidirectional tow is homogenised to a single orthotropic block. Multiaxial stressstrain response and degradation of material properties are modelled for unidirectional tows and º/9º laminates. BC: Matrix cracks CD & DE: (e) Wake debonding Matrix σ D Fibre A B C E CD & DE: Fibre rupture (f) DE: Fibre pullout (g) ν ν B D Figure. Schematic drawings of A unidirectional tow under longitudinal extension; and Longitudinal stressstrain and Poisson s ratiostrain curves; and (g) Corresponding damage modes. Poisson's ratio.... Experiment Idealisation Longitudinal strain Figure. Measured [8] and assumed variation of Poisson s ratios, ν and ν with longitudinal strain. DAMAGE MODES AND MECHANICAL BEHAVIOUR OF A UNI DIRECTIONAL TOW The damage modes and typical mechanical behaviour of a unidirectional tow subjected to different loading conditions are described in this section. The interactions of different damage modes and their effects on the stressstrain response are introduced.
3 Longitudinal extension When a unidirectional fibrereinforced ceramic matrix composite tow (single bundle of fibres and associated matrices) is under uniform extension along the fibre direction (Figure a), the typical longitudinal stressstrain response [5] (Figure b) and Poisson s ratiolongitudinal strain curve (Figure c), can be observed. The four characteristic stages in the stressstrain curve are now described [7]: AB: initially, the composite behaves as a virgin, undamaged, linear elastic material; BC: periodic matrix cracking occurs (Figure d); CD: fibrematrix interface debonding takes place at the matrix crack tip and its wake (wake debonding in Figure e); and weaker fibres fail (Figure f); DE: the majority of fibres fail and are pulled out against the frictional stress along the wake debonding interface (Figure g). Figure shows how the Poisson s ratiolongitudinal strain curve in Figure c can be idealised from the experimental data [8] for a unidirectional Nicalon/CAS composite. It can be seen that initially, Poisson s ratio is constant, then decreases linearly due to matrix cracking and wake debonding, and finally approaches zero at peak stress D, as shown in Figure b. σ A ν A B C B C To or Fibre Matrix debonding and/or matrix cracks (f) Figure. Schematic drawings of A unidirectional tow under transverse straining; and Transverse stressstrain and Poisson s ratio curves; and (f) Corresponding damage modes. γ γ τ A C B γ γ γ γ Fibre Matrix debonding and/or matrix cracks γ or (e) Figure 4. Schematic drawings of A unidirectional tow under shear straining; and Shear stressstrain curve; and (e) Corresponding damage modes.
4 Transverse extension When a unidirectional tow is subjected to transverse extension (Figure a), the material response is assumed to be piecewise linear elastic (Figure b and c). When the global transverse strain reaches a critical value, fibrematrix debonding and/or matrix cracking (Figure d f) is assumed to take place which leads to catastrophic failure. Shear loading As can be seen from Figure 4, in the case of shear straining, the shear stressstrain response and damage modes are assumed to have the same form as those for transverse straining. σ W Original N N W T W w w Nopullout Original Idealised Figure 5. Schematic drawing of Nopullout stressstrain curve; Variation of the normalised number of wake debonded blocks with longitudinal strain. Damage interactions and nopullout curve When a unidirectional tow is under multiaxial loading, e.g. both longitudinal and transverse straining ( and ); or both longitudinal and shear straining ( and γ ), the interaction between certain damage modes is strong and needs to be considered. The positive transverse stress ( σ ) or shear stress ( τ ) advances wake debonding, and hence decouples the interaction between fibres and matrix. As a result, the contribution due to fibre pullout has to be deactivated. Figure 5a shows that the original stressstrain curve degrades to the nopullout curve due to this damage interaction [5]. The damage interaction results in the change of Poisson s ratios. The broken curve in Figure 5b represents the variation of the normalised number of wake debonded blocks (fibrematrix between adjacent matrix cracks) in a tow with longitudinal strain [7]. In the present model, it is assumed that all the blocks wake debond at the point, W, viz. the dash curve in Figure 5b is idealised to the solid curve. The strain level at which the deactivation point W occurs has been determined by examination of the original and nopullout curves (Figure 5a). Consequently, Poisson s w ratios ν and ν drop to zero at the wake debonding strain,, when the switch to the nopullout curve is activated.
5 FORMULATION OF THE FINITE ELEMENT MODEL A unidirectional tow is chosen to be the basic constituent in the FE model, and therefore an entire tow, which consists of thousands of fibres embedded in matrix, can be represented by a single 8node solid finite element (Figure 6). The material properties are assumed to be multilinear elastic and the stressstrain and Poisson s ratiosstrain curves shown in Figures, and 4 are used to develop the constitutive equations. The FE package ABAQUS [9] with a userdefined subroutine UMAT is used to carried out the simulation. Tow Orthotropic Block This method has the benefit of being able to model a tow by a single orthotropic finite element. The approach has the advantage of simplicity relative to the binary system of modelling [5], since it has only one component; and, unlike the binary method, does not suffer from the difficulties associated with the identification of medium properties. Homogenisation of a unidirectional tow A heterogeneous unidirectional tow is homogenised to a single block (Figure 6), which has the same overall dimensions and equivalent orthotropic material properties. There are nine independent material properties: Young s moduli: E, E, and E ; Poisson s ratios: ν, ν, and ν ; Shear moduli: G, G, and G. Figure 6. Homogenisation of a unidirectional tow to a single orthotropic block. Discretisation of the stressstrain curve and constitutive equations In order to perform a finite element analysis, the nonlinear longitudinal stressstrain relationship is discretised to a multilinear curve. The loading is imposed in terms of the displacement boundary conditions, i.e. displacement controlled rather than load controlled conditions are modelled. The applied displacement is divided into many small increments. For each increment, the constitutive equations for an orthotropic material are: ν ν σ E E ν + ν ν σ E E σ = ν + ν ν τ EE τ τ ν + ν ν EE νν EE ν + νν EE ν + ν ν EE ν + νν EE νν EE G G γ γ γ G ()
6 ( ν ν ν ν νν ν ν ν ) E where = and ν i ij = ν ji (i, j = and i j). E E E E Assumptions of mechanical couplings due to damage interactions To model the interactions of the different damage modes, the following assumptions are made.. The switch from the original stressstrain curve to the nopullout curve is triggered by a small finite positive transverse stress, or by a small nonzero shear stress in the  or  plane.. Consequently, the Poisson s ratios, ν and ν drop to zero at the wake debonding strain, (Figure 5). w UMAT implementation in ABAQUS The present model is implemented by using the finite element package, ABAQUS/standard and a user defined subroutine, UMAT. The multilinear material properties, the constitutive equations, and the mechanical couplings are defined in the UMAT. For every increment, the UMAT reads the strains at each material point and then assigns the corresponding Young s moduli, Poisson s ratios and shear moduli. The constitutive equations are then used to update the stress fields. Solutiondependent state variables, STATEV, record different damage modes and control their interactions. Automatic incrementation algorithms and increment redefinition variable, PNEWDT, are continuously updated to ensure that the discretised points are located exactly at the end of the relevant increments. j MULTIAXIAL TOW AND º/9º LAMINATE BEHAVIOUR ( w,σ w ) σ σ D Wake debonding Longitudinal strain σ or σ Transverse strain or Poisson's ratio. ν. ν ν strain γ τ or γ τ γ τ Shear strain Figure 7. Material properties of a unidirectional tow.
7 The current model is used to analyse a unidirectional tow and a º/9º laminate under different loading cases. Applications to composite woven unit cells and real engineering components will be pursued as future developments. Material properties The material properties of a unidirectional tow of C/CSiC (Carbon/CarbonSilcon Carbide) DLRXT composite are shown in Figure 7. Figure 7a, which is associated with Figure 5a, has been obtained by using the model for a unidirectional tow [7]. The solid curve is the original longitudinal stressstrain relationship, the broken line defines the nopullout curve, and the cross symbol is the wake debonding point. The initial values of other properties, transverse moduli (Figure 7b), Poisson s ratios (Figure 7c), and shear moduli (Figure 7d) have been calibrated by a fully meshed micromechanical FE model. The limit of proportionality of the experimental stressstrain curve for the DLR XT material under uniaxial straining, is used to define a transverse failure strain of.4% []. A value of 6MPa is used to determine the critical shear failure strain []. Poisson's ratio Strain Longitudinal strain σ ν ν Poisson's ratio Strain Transverse strain σ ν ν Figure 8. Finite element results for a unidirectional tow under longitudinal straining ( ). Figure 9. Finite element results for a unidirectional tow under transverse straining ( ) Shear strain γ γ τ Figure. Finite element results for a unidirectional tow under shear straining.
8 Unidirectional tow: longitudinal, transverse and shear straining Figure 8 shows the FE results for a unidirectional tow under longitudinal straining. The stressstrain relationship, longitudinaltransverse strain curves, and variation of Poisson s ratios are plotted in Figure 8a, 8b, and 8c, respectively. As expected, the results are identical to the defined material properties. The results for a unidirectional tow subjected to transverse and shear straining are presented in Figures 9 and, respectively. Once again, the method has been validated since input and output values concur. Strain Strain ratio σ σ ( / ) Strain Strain ratio σ τ ( / ) ( / ) Longitudinal strain Longitudinal strain Figure. Finite element results for a unidirectional tow under equibiaxial straining ( = ). Figure. Finite element results for a unidirectional tow under longitudinal straining ( ) and shear straining (γ ) with =γ. Unidirectional tow: equibiaxial straining Figure shows the FE results for a tow under equibiaxial tensile straining, =. From Figure a, it can be seen that the nopullout stressstrain curve is triggered due to the positive stress σ. Figure b shows that the transverse stress, σ drops to zero at the defined failure strain ( =.4%). The effect of this transverse failure on the deformation in the other transverse direction is shown as a kink in Figure c. The
9 effect can also be seen from the first sharp drop in Figure d, which plots the ratio of strains in Figure c. The second sharp drop in Figure d is due to the second assumption of mechanical coupling, namely that the Poisson s ratio drops to zero at the wake debonding strain. Unidirectional tow: combined longitudinal and shear straining In comparison with the predictions for equibiaxial straining, similar results are obtained for longitudinal and shear straining (Figure ). In this case, the switch from original to nopullout curve is triggered by the shear stress. Transverse strains become zero at the wake debonding strain. º tows 9º tows Strain Composite strain σ Figure. Schematic drawing of a º/9º tow laminate under uniaxial straining Figure 4. Overall behaviour of a º/9º laminate under uniaxial straining Composite strain σ 9 σ Composite strain σ 9 σ Figure 5. Local behaviour of a º/9º laminate under uniaxial straining.
10 º/9º laminate under uniaxial straining, The model is also used to analyse a º/9º laminate under inplane uniaxial straining (Figure ). The overall stressstrain response and variations of transverse strains are shown in Figure 4a and 4b, respectively. The kinks at =.4% in both figures are due to the matrix cracking in the 9º tows. The transverse strains drop to zero at the wake debonding strain,. w Figures 5 show the longitudinal stressstrain and transverse stressstrain response in the different layers. As can be seen from Figure 5a, the nopullout curve is triggered in the º layer. This is because the º layer carries a transverse tensile stress (Figure 5c) before the wake debonding strain is reached. This tensile stress is created by the constraint of the 9º layer, since its stiffness in the direction is much higher than that of the º layer. In order to satisfy equilibrium, the transverse stress in the 9º layer (Figure 5d) is a mirror of that given in Figure 5c. According to this analysis, even though a º/9º laminate is only under inplane uniaxial tension, the nopullout curve can still be activated. This is different to the stressstrain response of longitudinal straining of a unidirectional tow. DISCUSSION AND CONCLUSIONS A computationally efficient FE model has been developed to predict the mechanical behaviour of ceramic matrix composites with straininduced damage. The effects of different damage modes and their interactions on mechanical behaviour have been considered. The basic constituent of the FE model is an orthotropic 8node brick, which forms a homogenised medium of a heterogeneous unidirectional tow. The nonlinear longitudinal material properties are discretised to a multilinear elastic curve. The constitutive equations for orthotropic materials are used to update the stresses for each increment of the analysis. The model is implemented by a commercial FE package, ABAQUS with a user defined subroutine, UMAT. Multiaxial stressstrain response and degradation of material properties have been modelled for a unidirectional tow, and for a º/9º laminate. In all analyses, the expected mechanical behaviour has been obtained. For the º/9º laminate under uniaxial straining, the nopullout stressstrain response in the º layer is triggered due to the constraint of the 9º layer. The high efficiency and the simplicity of the model make it possible to analyse large scale woven composites. Application of the model to unit cells and to real engineering components will be pursued as future developments. ACKNOWLEDGEMENTS Matthew Blacklock is gratefully acknowledged for providing the material properties used in this paper; and, for ongoing discussions.
11 References. Marshall, D. B. and Cox, B. N. 8 Integral textile ceramic structures. Annu. Rev. Mater. Res., 8, Sheikh, M. A., Taylor, S. C., Hayhurst, D. R. and Taylor, R. Microstructural finite element modelling of a ceramic matrix composite to predict experimental measurements of its macro thermal properties. Model. Simul. Mater. Sci. Eng. 9, 7.. Deepak, G. and Whitcomb, J. D. 8 Load flow in plain woven composites. Journal of Composite Materials. 4, Tanov, R. and Tabiei, A. Computationally efficient micromechanical models for woven fabric composite elastic moduli. Journal of Applied Mechanics. 68, Cox, B. N., Carter, W. C., and Fleck, N. A. 994 A binary model of textile composites I. Formulation. Acta Metall. Mater. 4, Hayhurst, D. R., Leckie, F. A. and Evans, A. 99 Component designbased model for deformation and rupture of tough fibrereinforced ceramic matrix composites. Proc. R. Soc. Lond. A. 44, Tang, C., Blacklock, M, and Hayhurst, D. R. 8 Thermomechanical behaviour of Ceramic Matrix Composites: Part I Stressstrain response and thermal conductivity degradation of fibre tows. Research report No. DMM. 8.4, School of Mechanical, Aerospace and Civil Engineering, The University of Manchester, U.K. 8. Karandikar, P. and Chou, T. 99 Characterization and modelling of microcracking and elastic moduli changes in Nicalon/CAS composites. Composites Science and Technology. 46, SIMULIA. 6 ABAQUS user s manual. Version Sheikh, M. A., Hayhurst, D.R., Taylor, S. C. and Taylor, R. 7 Experimental Investigation of the effect of mechanical loading on Thermal Transport in Ceramic Matrix Composites Research report No. DMM. 8.6, School of Mechanical, Aerospace and Civil Engineering, The University of Manchester, U.K.. Tang, C., Blacklock, M, and Hayhurst, D. R. 8 Thermomechanical behaviour of Ceramic Matrix Composites: Part II Stressstrain response and thermal conductivity degradation of fibre tows, 9 unidirectional and woven composites. Research report No. DMM. 8.5, School of Mechanical, Aerospace and Civil Engineering, The University of Manchester, U.K.
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationScienceDirect. Unit cell model of woven fabric textile composite for multiscale analysis. Anurag Dixit a *,Harlal Singh Mali b, R.K.
Available online at www.sciencedirect.com ScienceDirect Procedia Engineering 68 ( 2013 ) 352 358 The Malaysian International Tribology Conference 2013 (MITC2013) Unit cell model of woven fabric textile
More information3D Finite Element analysis of stud anchors with large head and embedment depth
3D Finite Element analysis of stud anchors with large head and embedment depth G. Periškić, J. Ožbolt & R. Eligehausen Institute for Construction Materials, University of Stuttgart, Stuttgart, Germany
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More information6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS
6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS Blondet et al. [25] carried out a cyclic test on an adobe wall to reproduce its seismic response and damage pattern under inplane loads. The displacement
More informationTransactions on Modelling and Simulation vol 10, 1995 WIT Press, ISSN X
Parameters controlling the numerical simulation validity of damageable composite toughness testing S. Yotte, C. Currit, E. Lacoste, J.M. Quenisset Laboratoire de Genie Meanique  IUT 'A\ Domaine Universitaire,
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationEffects of geometry and properties of fibre and matrix on overall. composite parameters
Int. Journal of Applied Sciences and ngineering Research, ol. 3, Issue 4, 2014 www.ijaser.com 2014 by the authors Licensee IJASR Under Creative Commons License 3.0 editorial@ijaser.com Research article
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationFINITE ELEMENT ANALYSIS OF THE ELASTIC CONSTITUTIVE BEHAVIOR OF A 2.5D INTERLOCK COMPOSITE
FINITE ELEMENT ANALYSIS OF THE ELASTIC CONSTITUTIVE BEHAVIOR OF A 2.5D INTERLOCK COMPOSITE NEHME Samer *, HAGEGE Benjamin *, KAABI Abderrahmen **, BENZEGGAGH Malk * * Université de Technologie de Compiègne,
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationDEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS
DEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS Mohsen Safaei, Wim De Waele Ghent University, Laboratory Soete, Belgium Abstract The present work relates to the
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationMATERIAL MECHANICS, SE2126 COMPUTER LAB 4 MICRO MECHANICS. E E v E E E E E v E E + + = m f f. f f
MATRIAL MCHANICS, S226 COMPUTR LAB 4 MICRO MCHANICS 2 2 2 f m f f m T m f m f f m v v + + = + PART A SPHRICAL PARTICL INCLUSION Consider a solid granular material, a so called particle composite, shown
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationFINITE ELEMENT ANALYSIS OF A LAYERED COMPOSITE CYLINDER USING THE CONNECTION BETWEEN THE MACRO AND MICROSTRUCTURE
FINITE ELEMENT ANALYI OF A LAYERED COMPOITE CYLINDER UING THE CONNECTION BETWEEN THE MACRO AND MICROTRUCTURE A. zekrényes Research Assistant, Department of Applied Mechanics, Budapest University of Technology
More informationBasic Energy Principles in Stiffness Analysis
Basic Energy Principles in Stiffness Analysis StressStrain Relations The application of any theory requires knowledge of the physical properties of the material(s) comprising the structure. We are limiting
More informationMechanics of Irregular Honeycomb Structures
Mechanics of Irregular Honeycomb Structures S. Adhikari 1, T. Mukhopadhyay 1 Chair of Aerospace Engineering, College of Engineering, Swansea University, Singleton Park, Swansea SA2 8PP, UK Sixth International
More informationThe Power of Ultrasonic Characterisation for Completely Assessing the Elastic Properties of Materials
11th European Conference on NonDestructive Testing (ECNDT 214), October 61, 214, Prague, Czech Republic The Power of Ultrasonic Characterisation for Completely Assessing the Elastic Properties of Materials
More informationPLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS PLAIN WEAVE REINFORCEMENT IN C/C COMPOSITES VISUALISED IN 3D FOR ELASTIC PARAMETRES P. Tesinova Technical University of Liberec, Faculty of Textile
More informationNigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37
Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREEDIMENSIONAL, TIME DEPENDENT, NONLINEAR, UNIDIRECTIONAL
More informationEXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS
EXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS Kevin L. Peil +, Ever J. Barbero +, Eduardo M. Sosa* + Department of Mechanical and Aerospace Engineering, West Virginia University (WVU), Morgantown,
More informationPlane Strain Test for Metal Sheet Characterization
Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and AnneMarie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS  Cachan, Avenue
More informationDon Robbins, Andrew Morrison, Rick Dalgarno Autodesk, Inc., Laramie, Wyoming. Abstract
PROGRESSIVE FAILURE SIMULATION OF ASMANUFACTURED SHORT FIBER FILLED INJECTION MOLDED PARTS: VALIDATION FOR COMPLEX GEOMETRIES AND COMBINED LOAD CONDITIONS Don Robbins, Andrew Morrison, Rick Dalgarno Autodesk,
More informationENGN 2290: Plasticity Computational plasticity in Abaqus
ENGN 229: Plasticity Computational plasticity in Abaqus The purpose of these exercises is to build a familiarity with using usermaterial subroutines (UMATs) in Abaqus/Standard. Abaqus/Standard is a finiteelement
More informationREPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 REPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
More informationPrediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads
Prediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads J. Raju 1*, D.S. Sreedhar 2, & C.M. Manjunatha 1 1
More informationVirtual tests based on model reduction strategies for fatigue analysis
Proceedings of the 7th GACM Colloquium on Computational Mechanics for Young Scientists from Academia and Industry October 1113, 217 in Stuttgart, Germany Virtual tests based on model reduction strategies
More informationA Critical Planeenergy Model for Multiaxial Fatigue Life Prediction. of Homogeneous and Heterogeneous Materials. Haoyang Wei
A Critical Planeenergy Model for Multiaxial Fatigue Life Prediction of Homogeneous and Heterogeneous Materials by Haoyang Wei A Thesis Presented in Partial Fulfillment of the Requirements for the Degree
More informationTHEME A. Analysis of the elastic behaviour of La Aceña archgravity dam
THEME A Analysis of the elastic behaviour of La Aceña archgravity dam Gjorgi KOKALANOV, Professor, Faculty of Civil Eng., Skopje, Republic of Macedonia Ljubomir TANČEV, Professor, Faculty of Civil Eng.,
More informationInvestigation of the Shear Thickening Fluid Dynamic Properties and its Influence on the Impact Resistance of Multilayered Fabric Composite Barrier
11 th International LSDYNA Users Conference Blast / Impact (1) Investigation of the Shear Thickening Fluid Dynamic Properties and its Influence on the Impact Resistance of Multilayered Fabric Composite
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationLectures on. Constitutive Modelling of Arteries. Ray Ogden
Lectures on Constitutive Modelling of Arteries Ray Ogden University of Aberdeen Xi an Jiaotong University April 2011 Overview of the Ingredients of Continuum Mechanics needed in Soft Tissue Biomechanics
More informationIMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS OBTAINED WITH LMS SAMTECH SAMCEF
V ECCOMAS Thematic Conference on the Mechanical Response of Composites COMPOSITES 015 S.R. Hallett and J.J.C. Remmers (Editors) IMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationA MULTISCALE MODELING APPROACH FOR THE PROGRESSIVE FAILURE ANALYSIS OF TEXTILE COMPOSITES MAO JIAZHEN NATIONAL UNIVERSITY OF SINGAPORE
A MULTISCALE MODELING APPROACH FOR THE PROGRESSIVE FAILURE ANALYSIS OF TEXTILE COMPOSITES MAO JIAZHEN NATIONAL UNIVERSITY OF SINGAPORE 2014 A MULTISCALE MODELING APPROACH FOR THE PROGRESSIVE FAILURE ANALYSIS
More information*Corresponding author: Keywords: Finiteelement analysis; Multiscale modelling; Onset theory; Dilatational strain invariant.
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MICROMECHANICAL MODELLING OF TEST SPECIMENS FOR ONSET OF DILATATIONAL DAMAGE OF POLYMER MATRIX IN COMPOSITE MATERIALS T. D. Tran 1, D. Kelly 1*, G.
More informationMECHANICAL BEHAVIOR OF WOVEN FABRIC COMPOSITES UNDER MESOLEVEL UNCERTAINTIES: MODELING AND SENSITIVITY ANALYSIS. Mojtaba Komeili
MECHANICAL BEHAVIOR OF WOVEN FABRIC COMPOSITES UNDER MESOLEVEL UNCERTAINTIES: MODELING AND SENSITIVITY ANALYSIS by Mojtaba Komeili B.Sc. Iran University of Science and Technology, Iran, 2008 A THESIS
More informationUse of negative stiffness in failure analysis of concrete beams
Use of negative stiffness in failure analysis of concrete beams A. Salam AlSabah Research Scientist, Debra F. Laefer Associate Professor* Urban Modelling Group, School of Civil Engineering, University
More informationTransactions on Engineering Sciences vol 13, 1996 WIT Press, ISSN
Computational debonding analysis of a thermally stressed fiber/matrix composite cylinder F.G. Buchholz," O. Koca* "Institute ofapplied Mechanics, University ofpaderborn, D33098 Paderborn, Germany ^Institute
More informationDETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1
PERIODICA POLYTECHNICA SER. CIV. ENG. VOL. 46, NO. 1, PP. 125 148 (2002) DETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1 Nándor LIEGNER Department of Highway and Railway Engineering
More informationMODELING SLABCOLUMN CONNECTIONS REINFORCED WITH GFRP UNDER LOCALIZED IMPACT
MODELING SLABCOLUMN CONNECTIONS REINFORCED WITH GFRP UNDER LOCALIZED IMPACT QI ZHANG and AMGAD HUSSEIN Faculty of Engineering, Memorial University of Newfoundland St. John s, Newfoundland, Canada, A1B
More informationEVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More informationMATERIAL MODELING OF STRAIN RATE DEPENDENT POLYMER AND 2D TRIAXIALLY BRAIDED COMPOSITES. A Dissertation. Presented to
MATERIAL MODELING OF STRAIN RATE DEPENDENT POLYMER AND 2D TRIAXIALLY BRAIDED COMPOSITES A Dissertation Presented to The Graduate Faculty of The University of Akron In Partial Fulfillment of the Requirements
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationDebonding process in composites using BEM
Boundary Elements XXVII 331 Debonding process in composites using BEM P. Prochazka & M. Valek Czech Technical University, Prague, Czech Republic Abstract The paper deals with the debonding fibermatrix
More informationNUMERICAL SIMULATIONS OF CORNERS IN RC FRAMES USING STRUTANDTIE METHOD AND CDP MODEL
Numerical simulations of corners in RC frames using StrutandTie Method and CDP model XIII International Conference on Computational Plasticity. Fundamentals and Applications COMPLAS XIII E. Oñate, D.R.J.
More informationMechanical Behavior of Fullerene Reinforced Fiber Composites with Interface Defects through Homogenization Approach and Finite Element Method
, pp.6782 http://dx.doi.org/1.14257/ijast.215.78.6 Mechanical Behavior of Fullerene Reinforced Fiber Composites with Interface Defects through Homogenization Approach and Finite Element Method P. Prasanthi
More informationMULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS
MULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS F.X. Irisarri, J.F. Maire* and N. Carrere ONERA, 9 av. de la Division Leclerc, 930 Châtillon, France francoisxavier.irisarri@onera.fr,
More informationTask 1  Material Testing of Bionax Pipe and Joints
Task 1  Material Testing of Bionax Pipe and Joints Submitted to: Jeff Phillips Western Regional Engineer IPEX Management, Inc. 20460 Duncan Way Langley, BC, Canada V3A 7A3 Ph: 6045348631 Fax: 6045347616
More informationFinite element analysis of diagonal tension failure in RC beams
Finite element analysis of diagonal tension failure in RC beams T. Hasegawa Institute of Technology, Shimizu Corporation, Tokyo, Japan ABSTRACT: Finite element analysis of diagonal tension failure in a
More informationAfter lecture 16 you should be able to
Lecture 16: Design of paper and board packaging Advanced concepts: FEM, Fracture Mechanics After lecture 16 you should be able to describe the finite element method and its use for paper based industry
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationNumerical Characterization of Concrete Heterogeneity
Vol. Materials 5, No. Research, 3, 2002Vol. 5, No. 3, Statistical 309314, 2002. Characterization of the Concrete Numerical Modeling of Size Effect In Heterogeneity 2002 309 Numerical Characterization
More informationUniversity of Bristol  Explore Bristol Research. Early version, also known as preprint
Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), 12291245. DOI: 10.1177/0021998305057432
More informationMultiple SpatioTemporal Scale Modeling of Composites Subjected to Cyclic Loading
Multiple SpatioTemporal Scale Modeling of Composites Subjected to Cyclic Loading Robert Crouch 1, Caglar Oskay 1, and Stephen Clay 2 1 Department of Civil and Environmental Engineering, Vanderbilt University,
More informationStress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole
Stress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole Dheeraj Gunwant, J. P. Singh mailto.dheerajgunwant@gmail.com, jitenderpal2007@gmail.com, AIT, Rampur Abstract A static
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More informationFRACTURE MECHANICS FOR MEMBRANES
FRACTURE MECHANICS FOR MEMBRANES Chong Li, Rogelio Espinosa and Per Ståhle Solid Mechanics, Malmö University SE 205 06 Malmö, Sweden chong.li@ts.mah.se Abstract During fracture of membranes loading often
More informationINFLUENCE OF WEB THICKNESS REDUCTION IN THE SHEAR RESISTANCE OF NONPRISMATIC TAPERED PLATE GIRDERS
INFLUENCE OF WEB THICKNESS REDUCTION IN THE SHEAR RESISTANCE OF NONPRISMATIC TAPERED PLATE GIRDERS Paulo J. S. Cruz 1, Lúcio Lourenço 1, Hélder Quintela 2 and Manuel F. Santos 2 1 Department of Civil
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationU.S. South America Workshop. Mechanics and Advanced Materials Research and Education. Rio de Janeiro, Brazil. August 2 6, Steven L.
Computational Modeling of Composite and Functionally Graded Materials U.S. South America Workshop Mechanics and Advanced Materials Research and Education Rio de Janeiro, Brazil August 2 6, 2002 Steven
More informationMODELLING OF DAMAGE IN TEXTILE REINFORCED COMPOSITES: MICRO MESO APPROACH
B. Van Den Broucke et.al., Modelling of damage in textile reinforced composites: micro meso approach MODELLING OF DAMAGE IN TEXTILE REINFORCED COMPOSITES: MICRO MESO APPROACH B. Van Den Broucke,2,, P.
More informationANALYSIS AND NUMERICAL MODELLING OF CERAMIC PIEZOELECTRIC BEAM BEHAVIOR UNDER THE EFFECT OF EXTERNAL SOLICITATIONS
Third International Conference on Energy, Materials, Applied Energetics and Pollution. ICEMAEP016, October 3031, 016, Constantine,Algeria. ANALYSIS AND NUMERICAL MODELLING OF CERAMIC PIEZOELECTRIC BEAM
More informationComputers and Geotechnics
Computers and Geotechnics 39 (212) 16 Contents lists available at SciVerse ScienceDirect Computers and Geotechnics journal homepage: www.elsevier.com/locate/compgeo Numerical analysis of the failure process
More informationPoisson s ratio as a sensitive indicator of (fatigue) damage in fibrereinforced plastics
10.1111/j.14602695.2007.01095.x Poisson s ratio as a sensitive indicator of (fatigue) damage in fibrereinforced plastics W. VAN PAEPEGEM, I. DE BAERE, E. LAMKANFI and J. DEGRIECK Ghent University, Department
More informationSize Effects In the Crushing of Honeycomb Structures
45th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics & Materials Conference 1922 April 2004, Palm Springs, California AIAA 20041640 Size Effects In the Crushing of Honeycomb Structures Erik C.
More informationInterfacial partial debonding and its in uence on the elasticity of a twophase composite
Mechanics of Materials 32 (2000) 695±709 www.elsevier.com/locate/mechmat Interfacial partial debonding and its in uence on the elasticity of a twophase composite S.F. Zheng, M. Denda, G.J. Weng * Department
More informationLowCycle Fatigue Crack Growth in Ti6242 at Elevated Temperature Rebecka Brommesson 1,a, Magnus Hörnqvist,2,b, and Magnus Ekh 3,c
LowCycle Fatigue Crack Growth in Ti6242 at Elevated Temperature Rebecka Brommesson 1,a, Magnus Hörnqvist,2,b, and Magnus Ekh 3,c 1,3 Department of Applied Mechanics, Chalmers University of Technology,
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationA multiscale approach for composite materials as multifield continua
Materials Science Forum Vols. 539543 (27) pp. 25512556 online at http://www.scientific.net (27) Trans Tech Publications, Switzerland A multiscale approach for composite materials as multifield continua
More informationInsitu local strain measurement in textile composites with embedded optical fibre sensors
Insitu local strain measurement in textile composites with embedded optical fibre sensors S. Daggumati, E. Voet, I. De Baere, W. Van Paepegem & J. Degrieck Ghent University, Department of Materials Science
More informationA NEW SIMPLIFIED AND EFFICIENT TECHNIQUE FOR FRACTURE BEHAVIOR ANALYSIS OF CONCRETE STRUCTURES
Fracture Mechanics of Concrete Structures Proceedings FRAMCOS3 AEDFCATO Publishers, D79104 Freiburg, Germany A NEW SMPLFED AND EFFCENT TECHNQUE FOR FRACTURE BEHAVOR ANALYSS OF CONCRETE STRUCTURES K.
More informationAN IMPORTANT PITFALL OF PSEUDOSTATIC FINITE ELEMENT ANALYSIS
AN IMPORTANT PITFALL OF PSEUDOSTATIC FINITE ELEMENT ANALYSIS S. Kontoe, L. Pelecanos & D.M. Potts ABSTRACT: Finite Element (FE) pseudostatic analysis can provide a good compromise between simplified
More informationADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF COMPOSITES
NAFEMS WORLD CONGRESS 13, SALZBURG, AUSTRIA ADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF M. Bruyneel, J.P. Delsemme, P. Jetteur (LMS Samtech, Belgium); A.C. Goupil (ISMANS, France). Dr. Ir. M. Bruyneel,
More informationFinite element simulation of residual stresses in laser heating
IAS200866546ST Finite element simulation of residual stresses in laser heating G. H. Farrahi 1, M. Sistaninia 2, H. Moeinoddini 3 1,2School of Mechanical Engineering, Sharif University of Technology,
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationMODEL VALIDATION AND STRUCTURAL ANALYSIS OF A SMALL WIND TURBINE BLADE
8th International DAAAM Baltic Conference INDUSTRIAL ENGINEERING 1921 April 2012, Tallinn, Estonia MODEL VALIDATION AND STRUCTURAL ANALYSIS OF A SMALL WIND TURBINE BLADE Pabut, O.; Allikas, G.; Herranen,
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationINFLUENCE KINDS OF MATERIALS ON THE POISSON S RATIO OF WOVEN FABRICS
ISSN 18466168 (Print), ISSN 18485588 (Online) ID: TG217816142553 Original scientific paper INFLUENCE KINDS OF MATERIALS ON THE POISSON S RATIO OF WOVEN FABRICS Željko PENAVA, Diana ŠIMIĆ PENAVA, Željko
More informationDynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models
Dynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models I. Rhee, K.J. Willam, B.P. Shing, University of Colorado at Boulder ABSTRACT: This paper examines the global
More informationContinuum Mechanics. Continuum Mechanics and Constitutive Equations
Continuum Mechanics Continuum Mechanics and Constitutive Equations Continuum mechanics pertains to the description of mechanical behavior of materials under the assumption that the material is a uniform
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More informationPractical methodology for inclusion of uplift and pore pressures in analysis of concrete dams
Practical methodology for inclusion of uplift and pore pressures in analysis of concrete dams Michael McKay 1 and Francisco Lopez 2 1 Dams Engineer, GHD Pty 2 Principal Dams/Structural Engineer, GHD Pty
More informationMultiscale modeling of failure in ABS materials
Institute of Mechanics Multiscale modeling of failure in ABS materials Martin Helbig, Thomas Seelig 15. International Conference on Deformation, Yield and Fracture of Polymers Kerkrade, April 2012 Institute
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More informationInterlaminar fracture characterization in composite materials by using acoustic emission
5th International Symposium on NDT in Aerospace, 1315th November 2013, Singapore Interlaminar fracture characterization in composite materials by using acoustic emission Ian SILVERSIDES 1, Ahmed MASLOUHI
More informationGeneric Strategies to Implement Material Grading in Finite Element Methods for Isotropic and Anisotropic Materials
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Engineering Mechanics Dissertations & Theses Mechanical & Materials Engineering, Department of Winter 1292011 Generic
More informationAE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF HOOP STRESSES FOR A THINWALL PRESSURE VESSEL
Objective AE3610 Experiments in Fluid and Solid Mechanics TRANSIENT MEASUREMENTS OF OOP STRESSES FOR A TINWA PRESSURE VESSE This experiment will allow you to investigate hoop and axial stress/strain relations
More information